# Semiconductor Device Reliability Failure Models

Embed Size (px)

### Transcript of Semiconductor Device Reliability Failure Models

Semiconductor Device Reliability Failure Models

International SEMATECHTechnology Transfer # 00053955A-XFR

© 2000 International SEMATECH, Inc.

SEMATECH and the SEMATECH logo are registered service marks of SEMATECH, Inc.International SEMATECH and the International SEMATECH logo are registered service marks

of International SEMATECH, Inc., a wholly-owned subsidiary of SEMATECH, Inc.

Product names and company names used in this publication are for identification purposes only and may be trademarks or service marks of their respective companies.

Semiconductor Device Reliability Failure ModelsTechnology Transfer # 00053955A-XFR

International SEMATECHMay 31, 2000

Abstract: No abstract.

Keywords: Reliability Modeling, Failure Mechanisms, Electromigration, Corrosion, Stress Migration

Authors: Richard Blish, Noel Durrant

Approvals: Noel Durrant, Program ManagerDave Anderson, Director, Supplier Relations & Corporate ServicesDan McGowan, Technical Information Transfer Team Leader

Page 1 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

SEMICONDUCTOR DEVICE RELIABILITY FAILURE MODELS

Abstract: This review paper brings together the most prevalent and important models for reliability failures insemiconductor devices. It gives a explanation of the failure, the failure model(s) and constraints of the models.Examples are presented showing the application of the models for deriving acceleration factors. Original referencesare included for each model.

Editors:Richard Blish, Advanced Micro DevicesNoel Durrant, Intel Corporation

Contributors:

Ted Dellin, SandiaDon Denton, Texas InstrumentsBabak Sabi, Intel CorporationDennis Eaton, AgilentPeng Fang, Advanced Micro DevicesSteve Huber, Intel CorporationJeff Kersey, Advanced Micro DevicesNick Lycoudes, MotorolaJack McCullen, Intel CorporationJoe McPherson, Texas InstrumentsTony Oates, Lucent TechnologiesPramod Patel, Advanced Micro DevicesCarl Peridier, Lucent TechnologiesGeorge Prokop, IBMTS Sriram, Compaq

Page 2 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

Table of Contents

Objectives, Scope and Explanation of Symbols............................................................................................................3

A. ELECTROMIGRATION..................................................................................................................................................4

B. CORROSION..................................................................................................................................................................7

C. TIME DEPENDANT DIELECTRIC BREAKDOWN........................................................................................................9

D. HOT CARRIER INJECTION .......................................................................................................................................12

E. SURFACE INVERSION (Mobile Ions) .......................................................................................................................14

F. STRESS MIGRATION..................................................................................................................................................16

G. TEMPERATURE CYCLING & THERMAL SHOCK ....................................................................................................19

H. SOFT ERRORS (Single Event Upsets) .....................................................................................................................22

I. Design of Experiments for Determination of Modeling Parameters.......................................................................24

J. Time-To-Failure Distributions....................................................................................................................................25

Page 3 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

OBJECTIVES, SCOPE AND EXPLANATION OF SYMBOLS

Objectives

� Provide critical assessment of best known models to predict Acceleration Factors (AF), FITs & DPM for common ICfailure mechanisms.

� Provide the SEMATECH Reliability Technology Advisory Board’s consensus-accepted method to calculate AF,FITs & DPM corresponding to specific failure mechanisms between reliability stress conditions and differentenvironmental conditions, e. g. office, mobile, or other market segment conditions.

� Provide literature citations to original, relevant source materials.� Provide numerical examples to illustrate how to apply these models.

Scope

This document covers most commonly observed integrated circuit failure mechanisms; is not intended to be all-inclusive. In the future, additional models will be added to this document to cover additional failure mechanisms.Better models, when available, will be added for the existing failure mechanisms.

This document applies to the following:1. aluminum alloy metallization (doped with small amounts of Cu and/or Si),2. refractory metal barriers with thin anti-reflective coatings,3. doped silica or silicon nitride interlayer dielectrics,4. poly silicon or “salicide” gates ( such as W, Ni & Co salicide to decrease resistivity),5. thin SiO2 gate dielectric6. Si with p-n junction isolation7. Packages, both wire bonded and C4, particularly fatigue failure and humidity/corrosion effects

Explanation of Symbols, Variables and Abbreviations

TF = time to failureAF = Acceleration Factor = TFcond2/ TFcond1

A0, B0, C0 = process/material-dependent constant or scaling factorsJ = current densityJcrit = critical (threshold) current density which must be exceeded before failure will occurN = current density, substrate current or Relative Humidity exponentEa = activation energyk = Boltzmann’s constant = 8.62 x 10-5 eV/ °KRH = Relative Humidity as % (100% = saturated)T = absolute temperature in oKelvinFIT = Failures-in-time expressed as failure per billion device hoursM1 = first metal layerM2 = second metal layer<j> = average current densityQcrit = critical charge for soft upset evente= charge of an single electron

Additional symbols and variables are defined in the paper at the point of usage.

Page 4 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

A. ELECTROMIGRATION

Due to momenta exchange between the current-carrying electrons and the host metal lattice, aluminum ions can drift inthe direction of the electron current. Due to the presence of flux divergence centers, vacancies start to cluster, clustersgrow into voids, and the voids can continue to grow until they block the current flow in the aluminum. Thus, the currentis forced to flow through the supporting barrier layer and/or capping layer; the resultant increase in resistance leads todevice failure. Since this is a mass conserving process, accumulations of the transported aluminum ions increase themechanical stress in supporting dielectrics, and may eventually cause fractures and shorts to occur.

Constraints and Limitations for EM in Long Metal Lines� For Al-alloy stripes, terminated by bonding pads and having no barrier metalization, the total time-to-failure is

dominated by nucleation and N is observed to be equal to 2.� For Al-alloy stripes on barrier metal and terminated by tungsten plugs, one may see both an incubation (nucleation)

period, dominated by N=2, and a resistance rise (drift period) dominated by N=1 or a blend of both currentexponents to produce an intermediate value. Larger N values can be observed if Joule heating is not properlyconsidered.

� Under high current density test conditions, unaccounted self-heating can produce apparent current densityexponents much greater than 2. Therefore, extreme care must be taken when extrapolating time-to-failure datafrom high to low current densities.

� The industry standard NIST bow-tie type EM test structure with simple bonding pad connections is grosslyinadequate for present multilevel metal systems and generally gives overly optimistic EM results relative to via-fedtest structures.

� EM kinetics for both lines & vias are different according to linewidth.� Via-fed test structures must be carefully designed to avoid resistance saturation & reservoir effects, which can

produce misleading t50 and σ values.� Industry standard NIST bow-tie type EM test structures with simple bonding pad connections are inadequate for

multilevel metal systems tending to give overly optimistic EM results relative to via-fed test structures.� For aluminum alloy lines terminated by bond pads and having no barrier metalization, the total time-to-failure is

dominated by nucleation and N is observed to be 2.� Under high current density test conditions, unaccounted for self-heating can produce apparent current density

exponents much greater than 2. Thus, extreme care must be taken when extrapolating time-to-failure data fromhigh to low current densities.

Constraints and Limitations for EM in Vias and ContactsElectromigration associated with vias and contacts must be investigated separately because they show characteristicsunlike single leads fed by bond pads. For example,� Vias can show different degradation rates depending on electron current flow direction (M2 to M1 versus M1 to M2)� Via degradation rate is strongly dependent on via structure, number of vias and layout� Via degradation may have a reservoir effect [1-2].� Silicide formation and barrier type are extremely important for in contact electromigration� Silicon (not Aluminum) may be the dominant diffusing species for contact failure [3-6].� Contact failure occurs by increased barrier metal resistance for an Al-alloy stripe on barrier metal and terminated

by tungsten plugs If no refractory barrier is present, failure time is controlled by the rate of drift of Al away from acontact, as junction spiking will be the dominant failure mechanism for transport of Si through the Al grains

� If self-heating is neglected, an apparent current density exponent much greater than 2 can be observed under highcurrent density test conditions. Thus, extreme care must be taken when extrapolating time-to-failure data taken athigh density to low current density.

ModelThe generally accepted Black model to describe time-to-failure (TF) takes the form [7-13]:

TF = A0 (J - Jcrit )-N exp (Ea /kT)In this model� J must be greater than Jcrit to produce failure,� failure criterion will be product-dependent, probably defined as the maximum tolerable increase in resistance for

the worst-case path

Page 5 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

� Jcrit = critical (threshold) current densityJcrit is inversely related to the Blech length for the line being evaluated, i. e.,Jcrit * Lcrit ≅ 6000 A/cm - for Al alloys this is typical (Lcrit , JL product is approximately constant)

� when test stripe length is ~60 µm, then Jcrit is comparable to normal EM stressing current densities near 1 MA/cm2

� in layered metal systems or for those with relatively coarse pitch (linewidth > ~1 µm) N = 2, corresponding to anincubation period, but generally one should use N =1 for for deep sub-micron technologies. It is noteworthy thatone may observe an apparent current density exponent of ~2 if Jcrit is taken as zero.

� Ea = 0.5 – 0.6 eV for Al and Al with a small percent of silicon� Ea = 0.7 – 0.9 eV for pure aluminum or aluminum/copper alloys

For unipolar current waveforms, J is the average current density < J > [14-15].

For bipolar waveforms a “sweep-back’ recovery action takes place and the effective current density J is described by J= (< J+ > - r ) < J- >, where < J+ > is the average of the positive polarity pulses and< J- > is the average of the negative polarity pulses. The recovery factor r has a value of at least 0.7.

Electromigration Numerical ExampleObjective: Calculate Acceleration Factor in a mobile environment versus an office environment.Assumptions:� Very long Al-Cu metalization stripes with large grain size vs line width (bamboo grain structure)� Mobile = 80 °C chip temperature inside the laptop� Office = 50 °C chip temperature inside the enclosure� Mobile & Office current density of 2.5 & 2.0 X 105 A/cm2 , respectively.

� J >> Jcrit

� Ea = 0.8 eV� N = 2

The ratio of the TF values will be:

AF = ratio of TF values, Office/Mobile = (JOffice /JMobile)-N exp [(Ea /k)(1/ TOffice -1/ TMobile)]

AF = (2.0/2.5) -2 exp [(0.8 eV /8.62 x 10 -5 eV/°K) × (1/{273 °K+50 °C}-1/{273 °K+80 °C})]

AF, Mobile/Office = 1.5 × 10 = 15

So moving from the hot, high current density Mobile environment to the cool, low current density Office environmentwill increase the TF value to 15X that of the previous value. Current density accounts for a factor of 1.5, whiletemperature accounts for a factor of 10, giving a 15x overall increase.

References1. C. Graas, H. Le, J. McPherson and R. Havemann, IEEE-IRPS Proceedings, p. 173 (1994).2. J. McPherson, H. Le and C. Graas, Microelectron. Reliab., Vol. 37, p. 1469 (1997).3. S. Vaidya, et. al., "Electromigration Induced Shallow Junction Leakage with Al/Poly-Si Metallization", J.

Electrochem. Soc., Vol. 130, p. 496 (1983).4. S. Vaidya, et. al., "Shallow Junction Cobalt Silicide Contacts with Enhanced Electromigration Resistance”, J. Appl.

Phys. Vol. 55, p. 3514 (1984).5. S. Steenwyk and E. Kankowski, "Electromigration in Aluminum to Ta-Silicide Contacts”, IEEE-IRPS Proceedings,

p. 30 (1986).6. J. Ondrusek, C. Dunn and J. McPherson, IEEE-IRPS Proceedings, p. 154 (1987).7. H. Huntington and A. Grone, J. Phys. Chem. Solids, Vol. 20, p. 76(1961).8. J. Black, IEEE Trans., Vol. ED-16 (No. 4), p. 338 (1969).9. F. d-Heurle and P. Ho, “Thin Films: Interdiffusion and Reactions,” John Wiley & Sons, p. 243 (1978).10. Blech, J. Appl. Phys., Vol. 74, p. 1203 (1976).11. R. Filippi, G. Biery and M. Wood, Mat. Res. Soc. Symp. Proc., Vol. 309, p. 141 (1993).12. R. Filippi, G. Biery and R. Wachnik, J. Appl. Phys., Vol. 78, p. 3756 (1995).13. A. Oates, IEEE-IRPS Proceedings, p. 164 (1996).14. J. Maiz, IEEE-IRPS Proceedings, p. 220 (1988).

Page 6 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

15. L. Ting, J. May, W. Hunter and J. McPherson, IEEE-IRPS Proceedings, p. 311 (1993).

Page 7 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

B. CORROSION

ULSI devices with aluminum or aluminum alloys with small percentages of copper and silicon metalization are subjectto corrosion failures [1-2]. Corrosion occurs in these metalization in the presence of moisture and contaminants.Corrosion failures are usually classified as one of two broad groups: bonding-pad corrosion or internal corrosion. Bondpad corrosion is more common because the die passivation does not cover the metalization in the bond pad locations.Internal corrosion (internal to the chip, away from the bond pads) is attributed to weakness or damage in the diepassivation, permitting moisture to reach the metalization.

Three industry-standard tests are used to accelerate corrosion failure mechanisms� 85/85 (85 °C and 85% Relative Humidity)� autoclave (or pressure cooker, usually ~ 2 atmospheres absolute pressure)� HAST (Highly Accelerated Stress Testing) -typically 85% RH with steam pressure > ambient pressure

Constraints and Limitations� Industry consensus is that the proper activation energy for aluminum corrosion is in the 0.7-0.8 eV range� There is not a consensus for the humidity dependence due to lack of data below 85% RH.� The relevant relative humidity (RH) is a local RH, the RH found at the interface between the silicon chip and the

package, which is not necessarily the ambient RH. If power dissipation is small, then ambient RH is approximatelythe same as local RH. If the power dissipation is large, stress tests may need to employ a duty cycle <100% [3,4]to align local and ambient RH values well enough to get meaningful data.

ModelsTo extrapolate accelerated corrosion test results to field use-conditions, four models are commonly used, all of whichare Eyring models (Eyring makes the practical assumption of mathematically separable, independent variables). Themodels use the product of an RH term, an applied voltage term & a temperature-based Arrhenius factor. Choice ofmodel is largely personal preference as we generally lack data over a broad enough range of variation in temperature,voltage and RH to discriminate one model from another on the basis of statistical fit. However recent work [5] suggeststhe Exponential Model may be the most effective. There is industry speculation that a voltage term is needed in thesemodels, but there are not yet supporting data to specify the term.

Reciprocal Exponential Model [6-9]

TF = C0 exp [b/RH] f(V) exp [ Ea /kT]

where:C0 = arbitrary scale factor,b = ~300Ea = 0.3 eV,f(V) = an unknown function of applied voltage

Power Law (Peck) Model [10],

originally for Al corrosion, but applied to other failure mechanisms with different N & Ea values

TF = A0 RH-N f(V) exp[Ea /kT]

where,A0 = arbitrary scale factorN = ~2.7,Ea = 0.7-0.8 eV (appropriate for aluminum corrosion with chlorides are present)f(V) = an unknown function of applied voltage

Exponential Model [5, 11,12]TF = B0 exp [ (-a ) RH] f(V) exp [Ea /kT],

where,

Page 8 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

B0 = arbitrary scale factor,a = 0.10 – 0.15 per %RH,Ea = 0.7- 0.8 eV,f(V) = an unknown function of applied voltage

A fairly recent comparison of four models [5] favored the exponential model with an “a” value of 0.12 – 0.15.

RH2 (Lawson) Model [13]TF = C0 RH2 f(V) exp [ Ea /kT]

where:C0 = arbitrary scale factor, (typical value 4.4 x 10-4)RH = Relative Humidity as % (100% = saturated),Ea = 0.64 eV,f(V) = an unknown function of applied voltage

Corrosion Numerical ExampleObjective: Calculate the Acceleration Factor for Al corrosion (on bond pads) due to chloride contamination comparingan office environment vs a HAST environment.

Assume� Office = 50 °C chip temperature & 10% RH inside the enclosure (same absolute humidity as room at 20

°C/50%RH) & applied voltage of 5 V� HAST environment is 130 °C & 85% RH inside the stress chamber & applied voltage is 6 V� Ea = 0.75 eV� Peck RH exponent = –2.7, which was experimentally determined for Al corrosion by Peck et al� Corrosion rate is linear with applied voltage

Thus, the ratio of the TF values will be:

AF, ratio of TF values, office/HAST = (RHoffice/RHHAST)

-2.7 × (Voffice/VHAST ) × exp[(Ea /k) × (1/ Toffice -1/ THAST)]

AF = (10/85) –2.7 × (6/5) exp [(0.75 eV /8.62 x 10 -5 eV/°K) × (1/{273 °K+50 °C}-1/{273 °K+130 °C})]

AF, office/HAST = 323 × 1.2 × 210 = 8.1 x 10+4 = 81,400

This indicates that by moving from a HAST environment to the office environment will increase TF (time to fail) value to81,000 times the accelerated stress (HAST) value, of which 300X is due to RH, 1.2X due to applied voltage and 250X isdue to temperature.

References1. G. Schnable and R. Keen, IEEE-IRPS Proceedings, p. 170 (1969).2. D. Peck, IEEE-IRPS Proceedings, p. 81 (1970).3. T. Ajiki, M.Sugumoto, H. Higuchi, and S.Kumada, "A New Cyclic Biased THB Test for Power Dissipating ICs, ”

IEEE International Reliability Physics Symposium Proceedings,, 1979, pp. 118-126.4. C. G. Shirley and C.E. Hong, "Optimal Acceleration of Cyclic THB Tests for Plastic Packages, "International

Reliability Physics Symposium Proceedings,, 1991, pp. 12-21.5. J. McPherson, G. Bishel and J. Ondrusek, Proceedings of Third Intern. Symp. on Corrosion and Reliability of

Electronic Materials and Devices, Electrochem. Soc., V. 94-29, p. 270 (1994).6. J. Gunn, R. Camenga and S. Malik, IEEE-IRPS Proceedings, p. 66 (1983).7. J. Flood, IEEE-IRPS Proceedings, pp. 95-99, 1972.8. N. Lycoudes, Solid State Technology, p. 53 (Oct. 1978).9. K. Stringy and A. Schelling, 31st ECC Proceedings, p. 238 (1981).10. D. Peck, IEEE-IRPS Proceedings, p. 44 (1986).11. C. Dunn and J. McPherson, J. Electrochem. Soc., p. 661 (1988).

Page 9 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

12. H. Koelmans, IEEE-IRPS Proceedings, p. 168 (1974).13. R. Lawson, British Telecom. Technol. J., Vol. 2, No. 2, p. 95 (1984).

C. TIME DEPENDENT DIELECTRIC BREAKDOWN

Time-Dependent Dielectric Breakdown (TDDB) is an important failure mechanism in ULSI devices. The dielectric failswhen a conductive path forms in the dielectric, shorting the anode and cathode. The two models widely used indescribing TDDB are field-driven (E-model) and current-driven (1/E - model).

Constraints and Limitations� These models are intended for application to SiO2 with thickness greater than approximately 40A (4 nm).� Accuracy of these models for thinner (silicon) oxide is unknown.� Models and parametric values to effectively model “hi K” oxides (based on materials or composites other than

silica) are unknown.� Recently, several low-field/long-term TDDB studies showed that TDDB data were described more effectively by the

E-Model than the 1/E model [1-5].� The E-model is now based on fundamental, physical parameters (not empirically fitted parameters) and fits TDDB

data more effectively than the 1/E model [6-8].� The good fit of the physics-based E-model to the low-field/long-term TDDB data strongly suggests electric field is

the dominant degradation driver at low stresses characteristic of customer applications, and that constant currentstress is not relevant to customer application.

E-Model [ 1-14 ]In the E-Model, the cause of low-field (< 10MV/cm) TDDB is due to field-enhanced thermal bond-breakage at thesilicon-silica interface. The E-field serves to reduce the activation energy required for thermal bond breakage andtherefore exponentially increases the reaction rate for failure. Time-to-failure, inverse to reaction rate, decreasesexponentially:

TF = A0 exp[ - γ Eox ] exp[Ea /kT]where:

A0 = arbitrary scale factor, dependent upon materials and process

γ = field acceleration parameter, is temperature dependent, γ(T) =a/kT where a is the effective dipole momentfor the molecule (see Note 1 below)

Eox = electric field across the dielectric in MV/cm. It must be voltage compensated for band bending if anaccumulation layer is formed, but no compensation is needed if an inversion layer is formed. Eox is the quotientof the compensated voltage & the oxide thickness, tox. Note that tox should be electrically or physicallymeasured.

Previous work [14] provides values for (∆H) 0 and "a" and shows that γ has a 1/T dependence. This means that theactivation energy reduces linearly with the electric field,

Ea = (∆H)0 - a Eoxwhere:

Ea = effective activation energy (eV). Ea may be nearly temperature-independent if several types of disturbedbonding states are present in the dielectric and the reaction rates are mixed during high-field and/or high-temperature TDDB testing.

(∆H) 0 = the enthalpy of activation for bond breakage in the absence of external electric field (~2.0 eV)

a = effective molecular dipole-moment for the breaking bonds which value is ~7.2 eÅ .

For intrinsic failures in SiO2 dielectrics of thickness < 100Å, γ ~ 2.5-3.5 Naperians per MV/cm (~1.1-1.5 decades perMV/cm) and Ea = 0.6-0.9 eV. For extrinsic defects, effective oxide thickness can be quite thin and therefore the

Page 10 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

effective field can be very high. This leads to the apparently lower activation energy of about 0.3 eV observed duringburn-in.

1/E – Model [ 15-18 ]The cause of TDDB, even at low fields, is postulated to be due to current through the dielectric by Fowler-Nordheim (F-N) conduction. F-N injected electrons (from the cathode) cause impact ionization damage of the dielectric as theyaccelerate through the dielectric. Additionally, when these accelerated electrons reach the anode, hot holes may beproduced which can tunnel back into the dielectric causing damage (hot-hole anode injection mechanism). The time-to-failure is expected to show an exponential dependence on the inverse electric field, 1/E:

TF = τo(T) exp [ G(T) / Eox ]where:

τo(T) = a temperature dependent prefactor, ~ 1 x 10-11 sec

G = field acceleration parameter, ~ 350 MV/cm with a weak temperature dependence

Eox = electric field across the dielectric in MV/cm. It must be voltage compensated for band bending if anaccumulation layer is formed, but no compensation is needed if an inversion layer is formed. Eox is the quotientof the compensated voltage & the oxide thickness, tox. Note that tox should be electrically or physicallymeasured.

TDDB Numerical Example Using the E-modelObjective: Calculate the Acceleration Factor for gate oxide failure by TDDB for an office environment (chip inside anenclosure) compared to a test structure in a highly accelerated environment.Assume� Office = 50 °C chip temperature & an electric field of 4 MV/cm inside the enclosure,� Accelerated means 300 °C & 8 MV/cm� γ value of 3 Naperians (logarithm) per MV/cm� Activation energy of 0.75 eV (approximate center of the nominal range for Ea.)

The ratio of the TF values will be:

AF, ratio of TF values, office/accelerated = exp[ - γ(Eoffice - Eaccel) × exp [(Ea /k) × (1/Toffice - 1/Taccel)]

AF = exp[-3/(MV/cm) ×{4 MV/cm –8 MV/cm}]exp[(0.75eV /8.62x10 -5 eV/°K) ×{1/(273 °K+50 °C)-1/(273 °K+300 °C)}]AF, office/accelerated stress = [1.60 × 10+5 ] × [1.27 × 10+5]= 2 x 1010

So moving from a highly accelerated test structure environment to office environment will increase TF (time to fail)value to 2 x 1010 times the accelerated stress value, of which 16,000 X is due to electric field and 12,700 X is due totemperature.-----------------------------------------------------------------------------------------------------------------------------------------------------Note 1: Many papers in the literature may use and plot base 10 (rather than base e) when expressing the fieldacceleration factor. One should be careful to note whether base 10 or natural base e is being used. Some authors, forclarity reasons, will write the field acceleration as decades per MV/cm to emphasize that the base 10 is being used orNaperians per MV/cm to emphasize that the natural base e is being used. Many authors, however, may notemphasize this distinction to the reader and the reader must be cautious. The conversion factor between base 10 andbase e is 2.3:1, i.e., γbase e = 2.3 * γbase 10 . In this document, the natural base e is assumed.

Page 11 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

References

1. K. Boyko and D. Gerlach, IEEE-IRPS Proceedings, p. 1 (1989).2. J. Suehle, P. Chaparala, C. Messick, W. Miller and K. Boyko, IEEE-IRPS Proceedings, p. 120 (1994).3. P. Charparala, J. Suehle, C. Messick and M. Roush, IEEE-IRPS Proceedings, p. 61 (1996).4. J. Suehle and P. Chaparala, IEEE Trans. Elect. Devices, p. 801 (1997).5. M. Kimura, IEEE-IRPS Proceedings, p. 190 (1997).6. J. McPherson, V. Reddy and H. Mogul, Appl. Phys. Lett., Vol. 71, p. 1101 (1997).7. J. McPherson and H. Mogul, Appl. Phys. Lett., Vol. 71, p. 3721 (1997).8. J. McPherson and H. Mogul, IEEE-IRPS Proceedings, p. 47 (1998).9. E. Anolick and G. Nelson, IEEE-IRPS Proceedings, p. 8 (1979).10. D. Crook, IEEE-IRPS Proceedings, p. 1 (1979).11. Berman, IEEE-IRPS Proceedings, p. 204 (1991).12. J. McPherson and D. Baglee, IEEE-IRPS Proceedings, p. 1 (1985).13. J. McPherson and D. Baglee, J. Electrochem. Soc., Vol. 132, p1903 (1985).14. J. McPherson, IEEE-IRPS Proceedings, p. 12 (1986).15. Chen, S. Holland and C. Hu, IEEE-IRPS Proceedings, p. 24 (1985).16. J. Lee, I. Chen and C. Hu, IEEE-IRPS Proceedings, p. 131 (1988).17. Moazzami, J. Lee and C. Hu, IEEE Trans. Elect. Devices, Vol. 36, p. 2462 (1989).18. K. Schuegraph and C. Hu, IEEE-IRPS Proceedings, p. 7 (1993).

Page 12 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

D. HOT CARRIER INJECTION

Hot carrier injection describes the phenomena by which carriers gain sufficient energy to be injected into the gate oxide[1-9]. This occurs as carriers move along the channel of a MOSFET and experience impact ionization near the drainend of the device. The damage can occur at the interface, within the oxide and/or within the sidewall spacer.Interface-state generation and charge trapping induced by this mechanism result in transistor parameter degradation,typically as switching frequency degradation rather than a “hard’ functional failure.

Constraints and Limitations� HCI-induced transistor degradation is well modeled by peak substrate-current for the n-channels and peak gate

current for the p-channels, at least for transistors at > 0.25 µm.• For sub-0.25 µm P-channel, the drive current tends to decrease like NMOS after hot carrier stress.• For sub-0.25 µm P-channel, worst case lifetime occurs at maximum substrate current stress. The TF model is the

same as N-channel.� The drive-currents for the n-channel transistors tends to decrease after HCI stressing, the p-channel drive current

tends to decrease.� The off-state leakage can increase dramatically [8], especially for initially high current-drive p-channels.� HCI-induced transistor degradation modeling seems to be accurate, but the extrapolation from transistor

degradation to circuit-level degradation is uncertain and should be the focus of future research efforts.� There is growing evidence that HCI physics may be starting to change at 0.25 µm and smaller, leading changing

worst-case stress conditions[5].� Precise voltage models (rather than substrate current or gate current) would be very useful.� HCI evaluations are almost always performed on test structures rather than products and done under dc

conditions, thus the calculated lifetime should be considered a Figure of Merit for process comparison.� A short “lifetime” observed with dc test structures does NOT imply unacceptable product performance under ac

conditions.� Typically, HCI degradation causes reduced circuit speed rather than catastrophic failure, although clearly a large

enough speed reduction can cause device failure.� For products where the substrate or gate current is unknown, large voltage acceleration is possible because gate

and substrate current are exponential to the reciprocal gate oxide electric field• There have been reports that the temperature dependent of substrate current has a positive activation energy

when Vcc is lower than 2.5V. The temperature dependent model for lower Vcc is still under investigation.

ModelsGenerally, degradation induced by HCI can be described by:

∆p = Atn

where:� p is the parameter of interest (Vt, gm, Idsat, etc.),� A = material dependent parameter� t = time� n = empirically determined exponent which is a function of stressing voltage, temperature and effective transistor

channel length

N-channel ModelN-channel devices use an Eyring model (which makes the practical assumption of mathematically separable andindependent variables):

TF = B(Isub )-N exp(Ea/kT)

where:B = arbitrary scale factor (function of proprietary factors like doping profile, sidewall spacing, dimensions, etc. )Isub = peak substrate current during stressingN = 2 to 4, typically 3Ea = -0.1 eV to -0.2 eV (note Ea is negative)

Page 13 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

P-channel ModelTF = B(Igate )

-M exp(Ea/kT)where:

B = arbitrary scale factor (function of proprietary factors, such as doping profiles, sidewall spacing dimensions,etc.)Igate = peak gate current during stressing.M = 2 to 4Ea = -0.1eV to -0.2eV (note this is a negative activation energy)

A “rough rule-of-thumb”, for the substrate current versus voltage dependence of P-channel devices ispeak substrate current doubles for each 0.5V increase in source-drain voltage (Vds).

HCI Numerical ExampleObjective: Calculate the Acceleration Factor for Hot Carrier Injection of an n-channel device for an office environmentversus a test structure accelerated environment.Assume

� Office = 50 °C chip temperature & substrate current of 1 µA� Accelerated conditions are -40 °C & 10 µA substrate current� N = 3� Ea = -0.15 eV

AF, the ratio of the TF values will be:

AF, ratio of TF values, office/accelerated = (Isub office / Isub accel)-N exp[ (Ea /k) × [1/ Toffice -1/ Taccel}

AF = (1µA /10 µA) -3 exp [(-0.15 eV /8.62 × 10 -5 eV/°K) ×{1/(273 °K+50 °C)-1/(273 °K-40 °C)}]

AF, office/accelerated stress = 1 × 10+3 * 8 = 8000

So moving from accelerated test structure environment to the office environment will increase TF (time to fail) value toby 8000 X of the accelerated stress value, of which 1000 X is due to substrate current and 8-fold is due to temperature.

References1. S. Aur, A. Chatterjee and T. Polgreen, IEEE-IRPS Proceedings, p. 15 (1988).2. E. Takeda, R. Izawa, K. Umeda and R. Nagai, IEEE-IRPS Proceedings, p. 118 (1991).3. E. Snyder, D. Cambell, S. Swanson and D. Pierce, IEEE-IRPS Proceedings, p. 57 (1993).4. J. Wang-Ratkovic, R. Lacoe, K. Williams, M. Song, S. Brown and G. Yabiku, IEEE-IRPS Proceedings, p. 312

(1997).5. G. LaRosa, F. Guarin, S. Rauch, A. Acovic, J. Lukaitis and E. Crabbe, IEEE-IRPS Proceedings, p. 282 (1997).6. J.T. Yue, ULSI Technology, McGraw-Hill, p. 657 (1996).7. P. Fang, J. Yue, and D. Wollesen, “A Method to Project Hot-Carrier-Induced Punch Through voltage Reduction for

Deep Submicron LDD PMOS FETs at Room and Elevated Temperatures“, IEEE-IRPS Proceedings, p. 131(1982).

8. C. Huang, T. Rost and J. McPherson, IEEE-IRW Final Report, p. 63 (1994).

Page 14 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

E. SURFACE INVERSION (Mobile Ions)

Mobile ions can contaminate semiconductor processing materials. In SiO2 they are very mobile even in the presence ofmodest electric fields (~ 0.5 MV/cm) and modest temperatures (100°C). An accumulation of drifted ions at the Si/SiO2

interface causes surface inversion leading to device failure [1-6].

Sodium and potassium are the usual suspects, simply because of high mobility and their natural abundance. In a gatestructure under bias, they can drift from the polysilicon (anode) to the silicon substrate (cathode). A buildup of positiveions at the Si/SiO2 interface inverts the surface and severely degrades the oxide isolation. Ionic drift in SiO2 gatedielectric can also cause premature TDDB. In the case of EPROMs, mobile-ion accumulation around the negatively-charged floating polysilicon can lead to data retention fails.

Devices showing isolation-leakage failures may recover during an unbiased high temperature bake. The bake causesa redistribution of the mobile-ions away from the accumulated Si/SiO2 interface or floating polysilicon in an EPROMdevice.

Constraints and LimitationsThe activation energy for mobile-ion diffusion depends on several factors including� the diffusing species,� the medium through which the mobile ions diffuse� the concentration of the contaminant

� For low concentrations, and if deep interfacial traps exist, then one may see deep interfacial-trap dominatedactivation energy of ~ 1.8 eV for Na+ diffusion through SiO2.

� If the concentration of Na+ is high, then all interfacial traps may be filled and a lower activation energy will beobserved (Ea ~ 0.75 eV for simple Na+ drift through SiO2 ).

ModelMobile ions are influenced by both electric field and temperature. One can use Eyring model for temperature and onewould compute the product of inverse to the ionic flux & an Arrhenius factor the time-to-failure (TF) described by:

TF = A (Jion)-1exp(Ea/kT)

A = material constant,Jion = <(eD0ρE/kT) - (D0∂ρ(x,t)/∂x)> is the average flow of ions

� (eD0ρE/kT) is the drift current� (D0∂ρ(x,t)/∂x is the back-diffusion component� E = electric field� e = charge on the electron� D0 = diffusion coefficient� ρ = density of mobile ions� <> represents the time- averaged value of the time-dependent quantities enclosed,

Ea = activation energy� depends upon the medium through which the ion must diffuse� for Na+ it ranges from 0.75 to 1.8 eV, with 1.0 eV being typical (0.75 eV for bulk silica)

Page 15 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

Mobile Ion Numerical ExampleObjective: Calculate the Acceleration Factor for surface inversion for an office environment compared to anaccelerated stress environment.Assume:� Baseline or office conditions are

� [Na+] = 1010/cm3

� electric field = 5 MV/cm� Office = 50 °C chip temperature

� Accelerated stress is� Temperature = 250 °C� [Na+] = 1017/cm3

� electric field = 8 MV/cm in the dielectric under stress� same distance & gradient in both cases� Ea = 0.75 eV

� First consider whether the drift or diffusion term is dominant for flux. Since D0 & concentration factors the same forboth drift and diffusion, the ratio [drift/diffusion] becomes (eE/kT)/(1/typical distance). Plugging in some nominalvalues (electric field = 6.5 MV/cm, temperature = 150 °C , characteristic distance = 10-4 cm) then the unit-less ratio is~10-7. This means the diffusion flux is far more important than the drift flux for this particular case and therefore theelectric field will not be a factor in calculating an acceleration factor

The ratio of the TF values will be:

AF (ratio of TF values, office/accelerated stress) = (Jion office/Jion accel)-1 exp([Ea /k](1/ Toffice - 1/ Taccel]

AF = (1010 /cm-3/1017 /cm-3) –1 exp ([0.75 eV /8.62 × 10 -5 eV/°K](1/(273 °K+50 °C)-1/(273 °K+250 °C))

AF(accelerated/office) = 1 × 10+7 * 3.2 × 10+4 = 3.2 × 10+11

Moving from accelerated stress environment (deliberate contamination and high electric field) to the office environmentwill increase the TF value to 3.2 × 10+11 times the accelerated stress value. A factor of 1 × 107 is due to flux(concentration) while a factor of 32,000 is due to temperature.

References1. J. McPherson, “Accelerated Testing,” Electronic Materials Handbook, Volume 1, Packaging,” ASM International

Publishing, p. 887 (1989).2. E. Schlegel, G. Schnable, R. Schwartz and J. Spratt, “Behavior of Surface Ions on Semiconductor Devices," IEEE

Transactions on Electron Devices, Vol. ED-15, 1968, pp. 973-979.3. E.H. Snow, A.S. Grove, B.E. Deal, and C.T. Sah, “Ion Transport Phenomenon in Insulating Films, “J. Appl. Phys.

Vol 36, p. 1664 (1965).4. E.H. Snow and B.E. Deal, “Polarization Phenomena and Other Properties of Phosphosilicate Glass Films on

Silicon,” J. Electrochem. Soc., Vol 113, p. 263 (1966)5. P. L. Hefley and J. McPherson, “The Impact of an External Sodium diffusion Source on the Reliability of MOS

Circuitry IEEE-IRPS Proceedings, p. 167 (1988).6. D.A. Stuart, “Calculations of Activation Energy of Ionic Conductivity in Silica Glass by Classical Methods, “J. Amer.

Ceramic Soc, “ p. 573 (1954).

Page 16 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

F. STRESS MIGRATION

The term stress migration describes the movement of metal atoms under the influence of mechanical-stress gradients.Generally, stress gradients can be assumed to be proportional to the applied mechanical stress. Little occurs until thestress exceeds the yield-point of the metalization. Then flux divergence associated with the metal movement causesvoids in ULSI metal leads. The resistance rise associated with the void formation can cause electrical failures [1-6].

The role of stress and stress relaxation is very important in the nucleation and growth of voids in aluminum-alloyinterconnects. Cu doping in the aluminum is somewhat effective in suppressing grain-boundary diffusion, but is muchless effective if the grain size is large compared to linewidth, i. e. bamboo leads, as one observes slit-like voidformation due to intra-grain diffusion.

Constraints and Limitations• This model applies to Aluminum alloys (doped with Cu and/or Si) only, there is insufficient data on pure copper at

this time.• There is currently no standard industry test for SM. Typically, long (> 1000 µm) and narrow (< 2 µm width) stripes

are stored (unbiased) at temperatures of 150-250oC for 1-2 K hr and then electrically tested for resistanceincreases or reduction in breakdown currents. Electromigration stressing is optional after SM baking.

• The SM baking temperature should be carefully selected because the maximum creep rate is generally in therange between 150-250oC. The maximum in the creep rate occurs due to the high stress but low mobility at lowtemperatures, and low stress but high mobility at high temperatures.

• Because the mechanical stress is temperature dependent, a straightforward determination of the diffusionalactivation energy is difficult to obtain. Generally Ea~0.5-0.6 eV is used for grain-boundary diffusion and ~ 1 eV forsingle-grain (bamboo-like) diffusion.

• The use of refractory metal barriers or layered metallization tends to nullify the severe damage caused by slit-likevoid formation in bamboo leads.

• Refractory metal layer acts as a redundant conductor, shunting the current and reducing the electrical resistancerise due to the void formation.

Mechanical Stress ModelThe time-to-failure (TF) can use an Eyring model, for which one computes the product of a power law on mechanicalstress & an Arrhenius factor [3]:

TF = Ao (σ) -n exp(Ea/kT)where:

σ = constant stress load,n = 2-3 for ductile metals,

n is usually ~5 if creep, thus implies T < Tm/2)Ea= 0.5 - 0.6eV for grain boundary diffusion, ~ 1 eV for single grain (bamboo-like) diffusion,

Thermomechanical Stress ModelIf the stress is generated by differing thermal expansion rates, then the stress is called as “thermomechanical stress”and is proportional to the change in temperature -

σ ∝ (∆T)

Therefore the time-to-failure can be written [ 3 ],

TF = B0 (T0 - T)-n exp(Ea/kT)

where:T0 = stress free temperature for metal ( approximate metal deposition temperature for aluminum)n = 2 – 3, ( ~5 if creep, thus implies T < Tm/2)Ea = 0.5 - 0.6eV for grain-boundary diffusion, ~ 1 eV for intra-grain diffusion

Page 17 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

Page 18 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

Stress Migration Numerical ExampleCalculate the Acceleration Factor for stress migration in an office environment compared to an acceleratedenvironment.

Assume• Office = 50 °C chip temperature inside the enclosure,• Accelerated stress temperature = 150 °C.• Ea = 0.55 eV,• n = 2.5• T0 = 250 °C• Use the thermomechanical stress model TF = B0 (T0 - T)-n exp(Ea/kT)

The ratio of the TF values will be:

AF (ratio of TF values, office/accelerated) = ((T0 - Toffice)/(T0- Taccel))-n exp ([Ea /k](1/ Toffice -1/ Taccel))

AF = ((300-50)/(300-150)) –2.5 exp ([0.55 eV /8.62 x 10 -5 eV/°K](1/(273 °K+50 °C)-1/(273 °K+150 °C))

AF(office/mobile) = 0.28 × 105 = 30X

So moving from the accelerated environment to the Office environment will increase the TF value to 30-fold that of theaccelerated stress value. Mechanical stress changes the TF value by 0.28 x (farther from stress-free temperature),while temperature TF by 105X the accelerated stress value.

References1. J. Klema, R. Pyle and E. Domangue, IEEE-IRPS Proceedings, p. 1 (1984).2. J. Yue, W. Fusten and R. Taylor, IEEE-IRPS Proceedings, p. 126 (1985).3. J. McPherson and C. Dunn, J. Vac. Soc. Technology B, p. 1321 (1987).4. J. Yue, Reliability Chapter, “ULSI Technology,” McGraw-Hill, p. 674, (1996)5. J. McPherson, “Accelerated Testing,” Electronic Materials Handbook, Volume 1 Packaging,” ASM International

Publishing, p887 (1989).

Page 19 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

G. TEMPERATURE CYCLING & THERMAL SHOCK

Fatigue failures can occur in ULSI devices due to temperature cycling and thermal shock. Permanent damageaccumulates during thermal cycling, accumulating each time the device undergoes a normal power-up and power-down cycle. Such cycles can induce a cyclical stress that tends to weaken materials [1- 9], and may cause a numberof different types of failures, including

� Dielectric/thin-film cracking� Lifted bonds� Fractured/broken bond wires� Solder fatigue (joint/bump/ball)� Cracked die� Lifted die

Constraints and Limitations� “Linearity” is assumed, modeling parameters are constant over range of interest (stress vs customer application)� Alternative methods are needed for reliability estimates (AF or FITs) under certain conditions such as

� if the temperature cycle range crosses a critical temperature, e.g. Tg (glass transition temperature of polymer)� if a material property changes dramatically over the temperature range of interest. For example the stress

relaxation rate of lead-based solders changes substantially near room temperature (see note below).

Coffin-Manson Model [1-2 ]For ductile materials, low-cycle fatigue data are described by the Coffin-Manson equation:

Nf = A0 [1/∆εp ] B

where:Nf = cycles to failureA0 = a material constant∆εΡ = plastic strain range (irreversible strain for one hysteresis loop, unitless)B = an empirically determined constant

Low cycle fatigue is defined as a stress condition in which hundreds or thousands of cycles cause failure, while highcycle fatigue would require millions of cycles. The Coffin-Manson model was originally developed for ductile materials(iron and aluminum alloys for aircraft), but has been successfully applied to brittle materials.

Modified Coffin-Manson Model [3]The standard Coffin-Manson equation works well, even for brittle material failures, where failure is dominated by crackinitiation and growth rather than simple plastic deformation. However, during a temperature cycle, not all of thetemperature range ∆T may be inducing plastic deformation. If a portion of the cycle, ∆T0, is actually in the elasticrange, then this should be subtracted from the total plastic strain range.

∆εΡ ∝ (∆T - ∆T0 ) β

Therefore, for temperature cycling with plastic deformation, the Coffin-Manson equation becomes:

Nf = C0 [ ∆T - ∆T0] -q {1}

where :Nf = Number of cycles to failureC0 = a material dependent constant∆T = entire temperature cycle-range for the device∆T0 = the portion of the temperature cycle range in the elastic regionq = the Coffin-Manson exponent, an empirically derived constant

If the elastic range (∆T0) is much smaller than the entire temperature cycle range (∆T), then it may be dropped withoutsignificant error being introduced (usual practice). Most failure mechanisms will show the same failure rate for slowtemperature cycling and for rapid thermal shock, but solder fatigue is a significant exception. Low melting point solders

Page 20 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

are used at temperatures in excess of Tmelting/2, so creep is significant & the mechanical properties are extremely time-sensitive. Conversely, strain rate for brittle materials (those with large q values) seems to be largely irrelevant.

Values for q for common ULSI materials are [4]: q valueductile metal, e.g., solder 1-3hard metal alloys / intermetallics (e.g. Al-Au) 3-5brittle fracture (e.g. Si & dielectrics : SiO2, Si3N4 ) 6-9

Temperature Cycling Numerical ExampleObjective: Calculate the Acceleration Factor for wire bond intermetallics due to temperature cycling in an officeenvironment compared to an automotive environment.Assume:� Office = once daily temperature changes of 20 °C� Automotive = 4 cycles per day with a change of 80 °C� q= 4� ∆T >> ∆T0

� Use Nf = C0 [ ∆T - ∆T0] -q

The ratio of the TF values will be:AF (ratio of Nf values per stress cycle, office/automotive) = (∆Toffice/∆Tauto)

-4

AF = (20/80) –4

AF(office/automotive per cycle) = 256 per cycle, but more cycles/day for automotive also

Comparative evaluation of an automotive environment to office environment shows a time to fail value 1000-fold that ofthe automotive value, of which 256-fold is due to temperature excursion difference, while 4X is from cyclic frequency.

If a critical temperature is crossed during each temperature cycle, at least four different approaches can be used.1 AF and FITs can be calculated for each zone where the modeling parameters are constant. Using available

data [4,7,8], the Coffin Manson exponent can be allowed to vary between the high and low temperature zones.2 The most commonly used method utilizes a Coffin-Manson exponent weighted over the temperature range.3 An alternative is to use the Norris-Lanzberg approach, which adds additional multiplicative terms. Factors are

a cyclic frequency factor as a power law (typ. with exponent ~1/3) and a mild Arrhenius-like temperaturedependence (typically using an "activation energy" of ~0.01 eV with highest vs lowest cyclic temperature.

4 Perhaps the best method, but the most labor-intensive, is to use Finite Element Analysis (FEA) to derive thevon Mises or maximum principal stresses to feed the simple Coffin-Manson equation {1}.

References1. L. Coffin, Jr., Met. Eng. Q., Vol 3, p. 15 (1963).2. S. Manson, “Thermal Stress and Low-Cycle Fatigue,” McGraw-Hill, New York, (1966).3. C.F. Dunn and J.W. McPherson, “Temperature Cycling Acceleration Factors in VLSI Applications,” IEEE-IRPS

Proceedings., p. 252 (1990).4. R. C. Blish, II “Temperature Cycling and Thermal Shock Failure Rate Modeling IEEE-IRPS Proceedings, p 110

(1997).5. H. Caruso and A. Dasgupta, “A Fundamental Overview of Accelerated-Testing Analytic Models,” 1998 Proc. of

Annual Rel. and Maintainability Symp.,” pp 389-393.6. J. McPherson, “Accelerated Testing,” Electronic Materials Handbook, Volume 1 Packaging,” ASM International

Publishing, p. 887 (1989).7. C. Y. Li, R. Subrahamanyan, J. R. Wilcox and D. Stone, “Damage Integral Methodology for Thermal and

Mechanical Fatigue of Solder Joints,” Solder Joint Reliability, Theory and Applications, ed. John H. Lau, 1991,pp. 261-288.

8. P. M. Hall, “Creep and Stress Relaxation in Solder Joints,” Solder Joint Reliability, Theory and Applications, ed.John H. Lau, 1991, pp. 306-332.

Page 21 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

9. K. C. Norris and A. H. Landzberg, “Reliability of Controlled Collapse Interconnections,” IBM J. R&D Vol. 13, 1969,pp. 266-271.

Page 22 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

H. SOFT ERRORS (SINGLE EVENT UPSETS)

Soft Errors (also called Single Event Upsets)

Soft errors in memory devices were first mentioned by May and Woods in 1978 [1]. A 5 MeV alpha particle impingingon a memory cell will produce 1.4 million electron-hole pairs in silicon to a depth of 25 µm. Minority carriers arecollected by the voltage across the depletion layer. If the number of collected carriers is greater than the Qcrit (criticalcharge -- charge necessary to determine cell state), the cell state will change resulting in a "soft" (reversible) error. Atutorial [2] in the IEEE Transactions on Reliability provides an excellent introduction to the subject.

To accurately determine the sensitivity of integrated circuits to radiation-induced soft errors or single event upsets(SEU), all sources of radiation must be accounted for. At terrestrial, Earth-based altitudes, the predominant sources ofradiation include both cosmic radiation and alpha particle radiation from radioisotopic impurities in the package andchip materials. An overall assessment of a device’s sensitivity to SEU/SER is complete ONLY when the alpha particlecomponent AND the cosmic radiation component have been considered.

Constraints and Limitations• The Qcrit value of memory devices of the 1970s, 1980 and early 1990s has changed from approximately 1 million

electrons (~'70) to ~10K electrons (~'99))• For alpha particle tests the test source should match the expected environment. For package impurities (ceramics,

glass, epoxy filler) the isotope impurities are Th232 and U238, so the alpha source should be Th232. For flip-chip andC4, the impurities are Po210 and Pb210. The preferred alpha source here is Am241. The alpha particle sourceshould always be MUCH larger than the sample to assure all alpha impinging angles are possible.

• For cosmic ray evaluation (terrestrial), neutron or proton sources of five to several hundred MeV should be used.These sources may be found at government, academic and medical facilities.

Cosmic rays (mainly high energy neutrons) at sea level are typically of little concern. CPUs in desktop computers runat a high enough Vcc that the Qcrit value is rarely exceeded by cosmic ray induced ionization. Cosmic ray intensity is 10times worse at 2 Km above sea level and reaches a peak of approximately 300 times sea level at 10 Km [3]. Laptopcomputers are at risk in use durning flights on commercial airlines, which typically fly at ~10 Km. The hazard todevices in laptop computers is further exacerbated by the smaller Qcrit value resulting from a low Vcc voltage used toreduce power consumption.

The effects of alpha particles can be ameliorated by shielding and purity, but there is little defense against cosmic rays,short of architectural change (redundant bits & Error Correction Code, ECC). There is a fine review by Ziegler et alencompassing entire January 1996 IBM Journal of Research and Development [3]. Further discussion of the effects ofcosmic ray neutrons and measurement techniques is contained in an article by McKee et al [6].

Evaluation for alpha particles has been done historically using Th232 or Am241 sources. A test method is described in aMIL-STD-883 procedure [5], but this will be supplanted by a new spec from JEDEC Committee 13.4 (letter ballotplanned q1 2000, reference number TBD). Cosmic ray evaluation has been performed at high elevation locations. Forexample, Leadville, Colorado cosmic ray intensity is approximately 13 times that of New York City [4]. Cosmic rayeffects can be simulated by an appropriate neutron source. Software programs are available for design simulations,but their accuracy is not yet proven.

ModelThe basic relation for soft error failure rate (SER) is:

SER = (OER/AF) x 109 FITSWhere:

OER is the observed error rate (errors/hour) on the test sample using an alpha source,AF is the acceleration factor for the setup.

A Curie is 3.7 x 1010 disintegrations per second, thus the source alpha particle emission is 0.1 x 10-6 Ci * 3.7 x 1010 or3700 alpha/sec. The source area is 0.322 π/4 or 0.08 cm2. Thus, the total source intensity is 3700/0.8 or 46,600 α/sec/cm2. The ambient alpha intensity is 0.001/3600 or 2.78 x 10-7 α/sec/cm2. The acceleration factor is the test alpha flux

Page 23 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

divided by the ambient alpha flux or in this example 46,600/2.78 x 10-7 or 1.68 x 1011. The SER of the device asnormally packaged would then be (1,000/1.68 * 1011) x 109 or approximately 6 FITs.

Numerical ExampleAn alpha particle test might use a 0.1 µCi Am241 source to test a device typically packaged in a plastic package. ASER (Soft Error Rate) of 1,000 errors per hour is observed. Common molding compounds have a measured alphaemission rate of 0.001 α/hour/cm2 and no die coating is used. The Am241 source is 1/8” (0.32 cm) in diameter. Whatwould be the Soft Error Rate in FITs of the device as normally packaged? Warning … this numerical exampleillustrates Mil 883 Method 1032 rather than the new JEDEC spec.

References1. May, Timothy C. and Woods, Murray H., "A New Physical Mechanism for Sift Errors in Dynamic memories," IEEE-

IRPS Proceedings, pp 33-40 (1978).2. Lantz, L., "Tutorial: Soft Errors Induced by Alpha Particles," IEEE Transactions on Reliability, Vol. 45, No. 2, June

1996.3. Ziegler, J.F. et al, "IBM Experiments in Soft Fails in Computer Electronics (1978 -- 1994)," IBM J. of Res. Develop.

No. 1, January 1996. Entire Issue is devoted to soft errors and associated topics.4. Ziegler, J.F, "Terrestrial Cosmic Ray Intensities," IBM J. of Res. Develop., Vol. 42, No. 1, January 1998.5. MIL-STD-883 -- Test Methods and Procedures for Microelectronics, Method 1032, Package Induced Soft Error

Test Procedure (Due to Alpha Particles).6. McKee, M.C., et al, "Cosmic Ray Neutron Induced Upsets as a Major Contributor to the Soft Error Rate of Current

and Future generation DRAMs," IEEE-IRPS Proceedings, pp 1-6 (1996).

Page 24 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

I.DESIGN OF EXPERIMENTS FOR DETERMINATION OF MODELING PARAMETERS

If the modeling parameters for a particular failure mechanism are not available in the literature or from internal sourcesor the parameters are uncertain, a designed experiment is needed to measure the appropriate constants. It isessential that a range of "over-stresses" be used to produce a statistically significant number of failures. Overstressconditions can be used to define technology margin and acceleration factors.

For example, assume that a failure mechanism is thermally activated, and follows a conventional Arrhenius model i.e.

ln(rate) ∝ (Q/k)*(1/T),

where Q = activation energy, k = Boltzmann’s constant and T = Absolute Temperature.

Plotting the data as ln(rate) versus the reciprocal temperature will produce a straight only if a single mechanism ispresent. In order to get a reasonably accurate Q value, the 1/T values should be far enough apart to modulate the ratesignificantly (at least several-fold, preferably as modulated over as many orders of magnitude as you can manage).

How much difference in temperature stress is needed? If the expected Q ~0.7 eV and the relevant temperature is near100 °C, every 20 °C change in temperature will change the rate by ~3-fold. So, ±20 °C will modulate the rate by ±3-fold. Similarly, every 40 °C change in temperature will change the rate by 9-fold with corresponds to ±40 °Cmodulating the rate by ±9-fold.

As a second example, assume the failure mechanism is some sort of mechanical fatigue, for which the conventionalmodel is Coffin-Manson. The rate (or time to failure) is proportional to strainpower and the usual surrogate for strain isthe swing in temperature (∆T) between hot and cold in temperature cycling or thermal shock.

Plotting the data as log(rate) vs log(∆T) (or perform a power law regression fit) , the slope is the power (Coffin-Mansonexponent). How much temperature swing will is needed? Let’s say you expect a Coffin-Manson exponent of 4 and therelevant temperature swing (∆T) is 100 °C. If your experiment were to explore ∆T values half as large and twice aslarge as the nominal 100 °C, the failure rate would be modulated by 24 = 16-fold, which would provide enough changeto determine the Coffin-Manson exponent more accurately than your initial guess. As above in the Arrhenius example,you want to perturb the rate by as much as possible without changing to a different failure mechanism (verified byfailure analysis).

As a third example, let’s consider that your failure mechanism is electrically activated, perhaps something similar toTDDB, for which the conventional model is the "E-model." Thus, ln(rate) is proportional to the difference in electric field(∆V/tox). Plotting the data as ln(rate) vs ∆V/tox will produce a straight line (or one could perform an exponentialregression fit), for which the slope is the γ value. How much modulation in ∆V/tox will you need to modulate the failurerate significantly? Let’s say you expect a γ value of 1 decade per MV/cm of electric field. Thus, changes in electricfield of ±1 MV/cm will modulate the failure rate by an order of magnitude. You might also want to modulate tox to see ifthe relevant stress is electric field or voltage. As above in the other examples, you want to perturb the rate by as muchas possible without changing to a different failure mechanism.

As a fourth and final example, let’s consider that your failure mechanism responds to two different stresses. Forexample, TDDB is sensitive to both temperature and voltage. The key design strategy is to assume that an Eyringmodel will work adequately (separable stresses). You now construct a "space" (temperature is one axis and voltage isthe other) and make sure that your stress conditions explore a constrained area of that space, using factorial design.Your initial DOE (Design Of Experiments) might employ a 2x2 or 3x3 "box" or perhaps a box/star. A particularly goodreference for all DOE, factorial design and statistics issues is "Statistics for Experimenters" by Box, Hunter & Hunter(Wiley).

Page 25 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

J. TIME-TO-FAILURE DISTRIBUTIONS

Models for the several failure mechanisms are well suited for calculation of acceleration factors between one stresscondition and another. The “hidden” assumptions that an acceleration factor is valid:� each distribution is a single population AND� the dispersion in failure times is the same for both stress conditions AND� the same cumulative percentage failures are to be compared� A “Stress to Fail” method is used to characterize and qualify the process or product, producing a statistically

significant number of valid failures from which the failure mechanism and root cause can be determined

Several different distributions can be used to model failure rate under appropriate circumstances:

An exponential distribution implies a constant failure rate, which is generally not true if the product is insufficientlyscreened, improperly Designed for Reliability or if the product is past the bottom of the “bathtub,” into wearout phase.The exponential distribution is simple, a good approximation and works well if there are very few or zero failures.

A Weibull distribution can be used to model “weakest link” and has two variants. The two parameter version derives acharacteristic life for 63% fail and a shape parameter, usually called β. The three parameter version for Weibull retainst63 and β, but adds an “delay time” corresponding to the time required to initiate defects, which may then propagateuntil they cause failure. The solder fatigue & some other communities traditionally use Weibull, but most of thesemiconductor community uses the lognormal distribution. There is a simple relationship to relate Weibull shapeparameter (β) to lognormal σ (β = 1.2/σ) over a wide range of cumulative percent failing (~100 ppm to 99.99%) [1, butbe advised that Wager’s tutorial contains a ln(10) error, see below]. Since substantially all real data sets show identicalcorrelation coefficient whether plotted as lognormal or 2 parameter Weibull, one can say that the choice is personalpreference. However, lognormal is the preferred distribution for most failure mechanisms (except solder fatigue, useWeibull instead) on the basis of mathematical simplicity, physical basis, intuitive basis (Gaussian, etc.) and ease ofuse. Excel, or equivalent, is a powerful tool for plotting and curve-fitting either lognormal or Weibull. On the otherhand, the Weibull distribution is mathematically complicated (nested logarithms), non-physical & not Gaussian.

The lognormal distribution is based on a normal distribution of failures vs logarithm of time. The characteristic fittingparameters are the time to 50% cumulative failure (t50) and sigma, a measure of the time dispersion of the failures (σ =ln (t50/t16)). The preferred, graphical way to extract parametric data is to use Excel to plot NORMSINV(cume % fail) asabscissa vs. natural logarithm of stress time as ordinate. Then a least squares fit of a straight line (in Excel: Chart, AddTrendline, Options, Show Equation & Correlation Coefficient) will provide slope = σ and intercept = ln(t50), Providing asingle distribution is present. The lognormal distribution is particularly well suited to changing failure rate, especially ifa large number of failures are available. The existence of many failures is NOT bad news from a modeling perspective(actually necessary!). In fact, large number of failures is also preferable for determination of the product’s Achille’sHeel, such that Continuous Improvement, successful Failure Analysis and Corrective Action(s) can be implemented.

A lognormal plot is a very effective way to see if single or multiple populations are present.Multiple populations are indicated if• a substantial curvature to the plotted data (poor correlation coefficient), or• a substantial change in slope, or• an offset on the time axis (an arrest in cume % fail over some considerable time period), or• subsequent failure analysis shows different failure modes/mechanisms.

ONLY if a single population is indicated, do the t50 and σ values have any physical significance. If multiple populationsare present, one must parse the data such that each distribution is a single “pure” mechanism, which will show superiorcorrelation coefficient (minimal divergence at the ends of the distribution) and no abrupt change in slope or offset.

A common example for multiple populations is that of the “defective subpopulation” [2]. A proportion of the total samplemay contain defects and the remaining product is immortal for the failure mechanism in question. The usual indicationfor this situation is a large sigma value. Typical sigma values are: ~0.5 for wearout; ~1.5 for defects; > ~4 forimproperly analyzed defective subpopulations. The key to successful analysis of a defective subpopulation is to makean estimate for the asymptotic value for complete failure of all defect-ridden product. An effective method to establishthe asymptotic value is to plot cume percent failing vs time or vs log time. The asymptotic value for cume % is the size

Page 26 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

of the defective subpopulation. To extract valid t50 & sigma values, one must recompute the cume percent failing withthe sample size for the defective subpopulation ONLY. Then proceed with a lognormal plot as described above.

Tips for interpretation of lognormal plots. The abscissa (cume percent failing) is non-linear in cume %, but is linear inunits of sigma. Thus, t50 corresponds to sigma = 0 (at the mean failure time), while t16 corresponds to sigma = -1 (oneunit below the mean), t2.3 corresponds to sigma = -2 (two units below the mean), t0.1 corresponds to sigma = -3, (threeunits below the mean), etc. The ordinate is ln (time), but most people find it difficult to convert ln (time) values back totime values, whereas it is much easier to think in base 10. Accordingly, it is convenient to pick the scale factor alongthe ordinate (ln(time)) in increments of 2.3. Thus, each time increment is an order of magnitude, as ln(10) = 2.302.

There are two commonly used ways to quote failure rate. FITs (defined as number of Failures In Time perbillion hours, American 109 hr, not British or European 1012 hr) and DPM (Defects Per Million over some stated timeperiod). FITs are a rate, while DPM is an integral of rate over time. For example, if your data suggest constant failurerate (very few failures) & you had 100 FITs (100 /109 hr) for 10K hr (~1 yr), then the DPM is simply the product of FITs& time, producing 10-3 in this example, 1000 DPM. If the failure rate is known to be changing with time, having beenmodeled by the lognormal or Weibull distribution, then the FIT value is the instantaneous slope of cum % fail vs time.

It is important to quote FITs or DPM to a known Upper Confidence Level, invariant with number failing and with60% as the commonly used value. However, some users specify 90% or 95% UCL. The chi-squared distribution,supported well by Excel, is an effective way to “level the playing field.”

Numerical ExampleLet’s assume your objective is to calculate when 0.1% of the product will fail based on knowledge of the mean time tofail and some measure of the time dispersion (constant failure rate, lognormal sigma or Weibull beta). Let’s furtherassume that your failure mechanism has been established to be well fitted by the lognormal distribution with a t50 = 100years and a sigma of 0.7 (natural logarithm of 2 to illustrate the point). Since sigma = ln(t50/t16), we know that every 2-fold shorter time will move the cum % fail down the normal curve by one unit (also called sigma, but a differentquantity). Thus, 16% cum fail (-1 sigma) will occur at 50 years; 2.3% cum fail (-2 sigma) will occur at 25 years; 0.13%cum fail (-3 sigma) will occur at 12.5 years. This scenario (low sigma characteristic of wearout such aselectromigration) supplies a reasonably acceptable time before an appreciable cum % fail is seen (taken as 0.1%here), but the situation is FAR more serious if the sigma value increases. For example, if the sigma value doubles to1.4, each “milestone” along the cum % fail curve will occur 4-fold earlier in time … PER STEP. Thus, 50% cum will stilloccur at 100 years for this scenario, while 16% cum occurs at 25 years, 2.3% cum at 6.25 years and 0.13% cum at1.56 years (4-fold sooner than if sigma were half the value!). Clearly, low sigma is indicative of more robust product,even if the t50 value is “good.”

So moving from a MTTF (Mean Time To Fail or t50) mentality to a “DPM” environment (when will the early fails occur &how many?) will produce results STRONGLY dependent on the lognormal sigma or Weibull beta (shape parameter)value, either of which is a measure of failure time dispersion.

Numerical ExampleLet’s assume your objective is to calculate FITs or DPM, given 0 fail from a sample of 2000 in HTOL (125 C for 24 hr),a use condition of 55C, a known acceleration factor of 50:1, and an elapsed time in the field application (use condition)of 1 year. Since we have no fails, we will assume the exponential distribution, for which the failure rate (FITs) isconstant. The chi-square value for “0” fails at 60% Upper Confidence Level is 0.93. 24 hr HTOL is equivalent to 1200hr in the customer use condition (AF=50:1), so FITs = # [email protected]%UCL/device-hr = 0.93/(2000*1200hr) = 381 FITs(rate). The DPM (integral) is simply the product of the rate * time, which is 381 10-9 /hr* 8760 hr = 3.4 DPM.

SummaryAcceleration Factors are fine for comparing performance under different environmental stresses, but fail to answerquestions about the time element. The most important question for a user is when will the first 1 ppm fail, when for 10ppm, when for 100 ppm, etc? Customers will typically NOT be most interested in t50, but rather more interested in theearly failure rate (impacts warrantee costs, customer perception, reputation, etc.). Some customers will prefer theintegral of failure rate to count the “dead bodies” for purposes of assessing the financial impact. Choice of the propermathematical distribution will affect the results and proper choice will be a function of the number failing in theaccelerated stressing or in the field application and whether the failure rate is constant, increasing (wearout), ordecreasing (infant mortality) with time.

Page 27 Semiconductor Device Reliability Failure Models

International SEMATECH Reliability Technology Advisory BoardTechnology Transfer #00053955A-XFR

References1. A. Wager, IRPS Tutorial, 19962. P.A. Tobias & D.C. Trindade, “Applied Reliability,” 2nd Ed. 19963. J. R. King, “Probability Charts for Decision Making” TEAM (803) 323-8843 (1971)

International SEMATECH Technology Transfer2706 Montopolis Drive

Austin, TX 78741

http://www.sematech.orge-mail: [email protected]